Figure 1 : Bonding Jig. Figure 2 : Shear Bond Test Set-Up. Dentin Bond Strength of Maxcem Elite Under Various Curing Modes H. Lu*, H. Bui, X. Qian, D. Tobia - Kerr Corporation, Orange, CA. 998. INTRODUCTION
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Figure 1: Bonding Jig
Figure 2: Shear Bond Test Set-Up
Dentin Bond Strength of Maxcem Elite Under Various Curing Modes
H. Lu*, H. Bui, X. Qian, D. Tobia - Kerr Corporation, Orange, CA
Self-adhesive resin cements combine the essential functions of an etchant, a primer/adhesive, and a luting cement into a single material, thereby combining the steps of etching, priming and cementing into one. This simplified cementation procedure results in significant time savings for the dental practitioner. The use of a self-adhesive resin cement should also make the restorative procedure less technique sensitive, reducing the occurrence of post-operative sensitivity because the smear layer is not removed and only one step cementation is involved.
Recently, a new dual-curable paste/paste self-adhesive resin cement, Maxcem Elite (Kerr), was introduced that offers enhanced adhesion to various dental substrates by incorporating GPDM adhesive monomer, an optimized resin matrix; a patented redox initiator system; and 4:1 ratio automixing delivery system. In addition to enhanced adhesive property, Maxcem Elite also offers exceptional color stability, translucency, and increased radiopacity.
Extracted human teeth were embedded in cold-cure acrylics. A set of six specimens were prepared for each group. A low speed diamond saw was used to remove the crown and expose the occlusal dentin. The dentin substrates were polished with 240-grit and then 600-grit SiC paper, rinsed thoroughly with water, and air dried for a few seconds.
Each prepared substrate was then held securely by a bonding jig (Ultradent Inc.) with a cylindrical mold ( = 2.38 mm). Maxcem Elite was condensed into the mold, directly onto the un-etched and un-primed dentin surface. The cement was allowed to cure in the following modes: (i) self-cure only; (ii) light-cure (for 30s) immediately without delay; (iii) light-cure after 2-minute delay; (iv) light-cure after 4-minute delay; (v) light-cure after 6-minute delay. The bonded specimens (n=6 for each group) were then stored in de-ionized water at 37ºC for 24 hours before being subjected to debonding on an Instron mechanical tester (Model 4467, Instron Corporation) in shear mode using a notched (semi-circular) edge at a crosshead speed of 1.0 mm/min. Shear bond strength values in MPa were calculated by dividing the peak load by the bonding area.
Statistical analysis was performed using One-way ANOVA and Bonferroni’s method for pair-wise comparison to determine significant differences among groups (p 0.05).
* Means with the same letter are not statistically different at p>0.05. Standard deviation for each group is
noted in parentheses.
To study the effect of various curing modes on the dentin shear bond strength of Maxcem Elite to determine if light-curing Maxcem Elite immediately after placement would negatively affect its bond strength.
Maxcem Elite had similar dentin shear bond strength (SBS) in self-cure mode and light-cure (for 30s) immediately without delay. Changing the delay time before light-cure, between 0 minutes to 6 minutes, did not affect the SBS. ANOVA analysis revealed that the dentin SBS of Maxcem Elite obtained under various curing modes were not statistically different (p > 0.05) from each other.
The similarity in dentin SBS of Maxcem Elite could be attributed to following contributing factors: (1) the incorporation of GPDM adhesive monomer for establishing a strong bond to tooth structure; (2) its optimized resin matrix system for enhanced wetting ability; and (3) its patented color-stable redox initiator system providing very efficient dark-cure mechanism.
The dentin shear bond strength of Maxcem Elite was not influenced by various curing modes. Light-curing Maxcem Elite immediately after placement does not negatively affect its dentin bond strength.
Maxcem Elite Kerr